# Temperature Coefficient of Frequency Modeling for CMOS ... Abstractâ€”CMOS-MEMS resonators,...

date post

14-Apr-2020Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of Temperature Coefficient of Frequency Modeling for CMOS ... Abstractâ€”CMOS-MEMS resonators,...

IEEE TRANSACTIONS ON ULTRASONICS, FERROELECTRICS, AND FREQUENCY CONTROL, vol. 62, no. 6, JUNE 20151166

0885–3010 © 2015 IEEE. Personal use is permitted, but republication/redistribution requires IEEE permission. See http://www.ieee.org/publications_standards/publications/rights/index.html for more information.

Temperature Coefficient of Frequency Modeling for CMOS-MEMS Bulk Mode

Composite Resonators Siping Wang, Student Member, IEEE, Wen-Chien Chen, Member, IEEE,

Bichoy Bahr, Student Member, IEEE, Weileun Fang, Member, IEEE, Sheng-Shian Li, Member, IEEE, and Dana Weinstein, Member, IEEE

Abstract—CMOS-MEMS resonators, which are promising building blocks for achieving monolithic integration of MEMS structure, can be used for timing and filtering applications, and control circuitry. SiO2 has been used to make MEMS reso- nators with quality factor Q > 10 ,4 but temperature instability remains a major challenge. In this paper, a design that uses an embedded metal block for temperature compensation is pro- posed and shows sub-ppm temperature stability (−0.21 ppm/K). A comprehensive analytical model is derived and ap- plied to analyze and optimize the temperature coefficient of frequency (TCF) of the CMOS-MEMS composite material resonator. Comparison with finite element method simulation demonstrates good accuracy. The model can also be applied to predict and analyze the TCF of MEMS resonators with arbi- trary mode shape, and its integration with simulation packages enables interactive and efficient design process.

I. Introduction

Vibrating micromechanical resonators capable of providing high Q and zero dc power consumption have been implemented for timing references in a variety consumer electronics [1] [2]–[4], leading to smaller size and lower cost compared with conventional electrical components, such as crystal [5], [6], SAW [7], and film bulk acoustic resonator (FBAR) [8] resonators. Neverthe- less, the discrete nature of these off-chip micromechanical resonators still impedes the system miniaturization and circuit integration for future multiband, multimode wire- less transceivers [9], vibrational inertial sensors [10], and timing references [11], [12]. To realize MEMS resonators monolithically integrated with circuitry, in recent years CMOS-MEMS resonator platforms based on a foundry- oriented 0.35 μm 2-poly-4-metal (2P4M) CMOS technol- ogy [13]–[15] and 0.18 μm 1-poly-6-metal (1P6M) CMOS process [16], [17] have been developed to fabricate inte- grated vibrating micromechanical structures side by side

with circuits. However, due to the limited structural ma- terial option (i.e., metal and oxide) in CMOS technology, CMOS-MEMS resonators are mostly made of metal-rich structures, suffering relatively low Q and poor thermal stability [15], as compared with conventional silicon- based resonators. To solve the low-Q issues resulting from metal, a square plate oxide resonator composed of sili- con dioxide (SiO2) with embedded metal electrodes via a CMOS 0.18 μm process and a metal etching technique has been successfully developed with resonator Q exceed- ing 10 000 [18], as shown in Fig. 1. But this design has poor thermal stability due to the oxide-rich structure, which has a positive temperature coefficient of Young’s modulus (+TCE) [19].

To address thermal stability of capacitively transduced resonators, researchers have demonstrated passive tem- perature compensation techniques, such as the stress in- duced frequency compensation [20], composite structures consisting of silicon dioxide [21]–[23], and degenerate dop- ing [24]–[26], without consuming excessive power [27] or requiring complicated active compensation parabolic-type control circuits [28], [29]. Among these passive approach- es, composite structures consisting of silicon dioxide have recently become mainstream to achieve first-stage tem- perature compensation; because it is easy to process and has TCE of opposite sign relative to most other materi- als commonly used in CMOS-MEMS, it can thus be used to negate the temperature dependence of other materials. However, the temperature coefficient of frequency (TCF) for complicated composite structures can be difficult to control and predict analytically, leading to time-consum- ing simulations and a nonintuitive design process. In this work, we propose an analytical model for TCF based on perturbation theory capable of analyzing composite and unreleased structures with arbitrary material distribution and suitable for arbitrary composite material resonators. The model greatly accelerates the simulation process in- volved in designing a thermally stable resonant structure. As will be shown, the first-order TCF can be lowered from high positive value (+93 ppm/K) without compensation to sub-ppm level (−0.28 ppm/K) with the proposed com- pensation (according to simulation). The latter meets the requirement of high performance micromechanical oscil- lator for future timing devices or frequency synthesizer applications.

Manuscript received October 10, 2014; accepted March 14, 2015. S. Wang and W.-C. Chen contributed equally to this work. S. Wang, B. Bahr, and D. Weinstein are with the Department of

Electrical Engineering and Computer Science, Massachusetts Institute of Technology, Cambridge, MA 20139, USA (e-mail: spinwang@mit.edu).

W.-C. Chen, W. Fang, and S.-S. Li are with National Tsing Hua Uni- versity, Hsingchu, Taiwan.

From mid-2012 to mid-2013, W.-C. Chen was with Prof. Dana Wein- stein at the Massachusetts Institute of Technology, Cambridge, as a Vis- iting Student.

DOI http://dx.doi.org/10.1109/TUFFC.2014.006724

wang et al.: temperature coefficient of frequency modeling of composite resonators 1167

II. Modeling of Temperature Coefficient of Frequency

To demonstrate the ability to tune the thermal stabil- ity of bulk mode resonators, an oxide (+TCE) structure is embedded with metal (−TCE) blocks using CMOS- MEMS technology, achieving passive temperature com- pensation. This leads to the possibility of achieving a CMOS-MEMS resonator with high-Q as well as low TCF. A 0.18-μm 1-poly-6-metal standard CMOS process with diverse structural configuration and flexible material op- tion is utilized to construct the composite bulk acoustic Lamé mode resonator. The resonator can be modeled as the parallel combination of multiple square plates made of different material compositions as shown in Fig. 2, and each of these plates can be treated as a separate Lamé mode resonator. The thickness of mat.1 (hmat.1) and mat.2 (hmat.2) is 0.53 and 0.85 μm, respectively, and the plate side length is 22.95 μm. Driving and sensing capacitors have a gap size of 0.42 μm. Anchors are draw to scale in Fig. 2. Because layer thickness h is small compared with resonator side length, plane stress approximation is used and vibration is assumed to be 2-D only, with no depen- dence on the thickness dimension. The structure is com- posed of 3 types of plates: a metal-based plate embedded with oxide blocks (mat.1), an oxide-based plate embedded with metal blocks (mat.2), and one made purely of oxide (oxide). The embedded metal electrodes and oxide edge for etching protection [18] are neglected for a simplified illustration of the model, but will be included in the re- ported TCF of the final design. The overall linear TCF of the composite body is given as a linear combination of the TCFs of each single layer plate, as shown in (1). Detailed derivation is provided in Appendix A.

TCF TCF TCF TCFmat.1 mat.2 ox=

A B C A B C

⋅ + ⋅ + ⋅ + +

, (1)

where

A h f= 2mat.1 mat.1 mat.1ρ , (2)

B h f= 2 2 22mat. mat. mat.ρ , (3)

C h f= 2ox ox oxρ . (4)

In the above expressions, for a particular plate of type “mat,” TCFmat is the TCF calculated for each single layer, hmat is the layer thickness, fmat is the resonant frequency of that single layer plate, and ρmat is the plate’s effective density,

ρ ρ

mat = ( , ) ( , )

( , ) ,

2

2 Ω

Ω

Ω

Ω

∫ ∫ x y u x y

u x y

d

d (5)

where Ω represents resonator’s spatial domain. The thick- ness of each layer is defined by the foundry, and thus hmat is known from the design. TCFmat and fmat are variables dependent on the design, namely, embedding of compen- sating material. A fast analytical model for deriving these values given a certain design is the focus of the rest of this paper.

The overall TCF of a multilayer composite resonator can be calculated if the resonant frequency and TCF of each type of single layer plate are known. In this section, an analytical model for predicting the resonant frequencies and TCF of a generalized composite bulk acoustic resona- tor is presented. This analytical model lays the foundation for calculating and optimizing the TCF of the aforemen- tioned multilayer CMOS-MEMS resonator, but it can also be applied to quickly calculate the TCF of any MEMS resonator given its material composition and mode shape. For this particular multilayer CMOS-MEMS resonator, as will be shown in Section III, all the variables needed to calculate the overall TCF of the multilayer composite ma- terial resonator can be derived based on the unperturbed 2-D Lamé mode shape and material properties using this analytical model.

Fig. 1. A CMOS-MEMS Lamé mode resonator composed of SiO2, dem- onstrating Q > 104.

Fig. 2. Composite material mulitlayer Lamé mode CMOS-MEMS resona- tor for temperature compensation. The structure can be viewed as the parallel combination of 9 single layer

Recommended

*View more*